General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.4 g/cm³ Show Material materials with Density of 8.4 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 221 GPa Show Material materials with Elastic modulus of 221 GPa |

100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

200.0 °C | 211 GPa Show Material materials with Elastic modulus of 211 GPa | |

300.0 °C | 204 GPa Show Material materials with Elastic modulus of 204 GPa | |

400.0 °C | 197 GPa Show Material materials with Elastic modulus of 197 GPa | |

500.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | |

600.0 °C | 182 GPa Show Material materials with Elastic modulus of 182 GPa | |

700.0 °C | 174 GPa Show Material materials with Elastic modulus of 174 GPa | |

800.0 °C | 165 GPa Show Material materials with Elastic modulus of 165 GPa | |

900.0 °C | 154 GPa Show Material materials with Elastic modulus of 154 GPa | |

1000.0 °C | 140 GPa Show Material materials with Elastic modulus of 140 GPa | |

Elongation | 20.0 °C | 30 % Show Material materials with Elongation of 30 % |

Hardness, Brinell | 20.0 °C | 230 [-] Show Material materials with Hardness, Brinell of 230 [-] |

Tensile strength | 20.0 °C | 650 - 850 MPa Show Material materials with Tensile strength of 650 - 850 MPa |

Yield strength Rp0.2 | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp0.2 of 240 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.17E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.17E-5 1/K | |

200.0 °C | 1.26E-5 - 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.26E-5 - 1.27E-5 1/K | ||

300.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | ||

400.0 °C | 1.38E-5 - 1.39E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.38E-5 - 1.39E-5 1/K | ||

500.0 °C | 1.43E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.43E-5 1/K | ||

600.0 °C | 1.48E-5 - 1.5E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.48E-5 - 1.5E-5 1/K | ||

700.0 °C | 1.54E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.54E-5 1/K | ||

800.0 °C | 1.6E-5 - 1.65E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.65E-5 1/K | ||

900.0 °C | 1.66E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.66E-5 1/K | ||

1000.0 °C | 1.75E-5 - 1.82E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.82E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 1150 °C Show Material materials with Max service temperature, long of 0 - 1150 °C | ||

Melting point | 1400 °C Show Material materials with Melting point of 1400 °C | Typical for Nickel Chromium Alloy | |

Specific heat capacity | 20.0 °C | 445 - 460 J/(kg·K) Show Material materials with Specific heat capacity of 445 - 460 J/(kg·K) | |

100.0 °C | 465 J/(kg·K) Show Material materials with Specific heat capacity of 465 J/(kg·K) | ||

200.0 °C | 490 J/(kg·K) Show Material materials with Specific heat capacity of 490 J/(kg·K) | ||

300.0 °C | 515 J/(kg·K) Show Material materials with Specific heat capacity of 515 J/(kg·K) | ||

400.0 °C | 540 J/(kg·K) Show Material materials with Specific heat capacity of 540 J/(kg·K) | ||

500.0 °C | 570 J/(kg·K) Show Material materials with Specific heat capacity of 570 J/(kg·K) | ||

600.0 °C | 600 J/(kg·K) Show Material materials with Specific heat capacity of 600 J/(kg·K) | ||

700.0 °C | 620 J/(kg·K) Show Material materials with Specific heat capacity of 620 J/(kg·K) | ||

800.0 °C | 650 J/(kg·K) Show Material materials with Specific heat capacity of 650 J/(kg·K) | ||

900.0 °C | 675 J/(kg·K) Show Material materials with Specific heat capacity of 675 J/(kg·K) | ||

1000.0 °C | 700 J/(kg·K) Show Material materials with Specific heat capacity of 700 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 12 - 12.1 W/(m·K) Show Material materials with Thermal conductivity of 12 - 12.1 W/(m·K) | |

100.0 °C | 13.7 W/(m·K) Show Material materials with Thermal conductivity of 13.7 W/(m·K) | ||

200.0 °C | 15.6 W/(m·K) Show Material materials with Thermal conductivity of 15.6 W/(m·K) | ||

300.0 °C | 17.1 W/(m·K) Show Material materials with Thermal conductivity of 17.1 W/(m·K) | ||

400.0 °C | 18.8 W/(m·K) Show Material materials with Thermal conductivity of 18.8 W/(m·K) | ||

500.0 °C | 20 - 20.5 W/(m·K) Show Material materials with Thermal conductivity of 20 - 20.5 W/(m·K) | ||

600.0 °C | 22.6 W/(m·K) Show Material materials with Thermal conductivity of 22.6 W/(m·K) | ||

700.0 °C | 24.5 W/(m·K) Show Material materials with Thermal conductivity of 24.5 W/(m·K) | ||

800.0 °C | 26.4 W/(m·K) Show Material materials with Thermal conductivity of 26.4 W/(m·K) | ||

900.0 °C | 28.1 W/(m·K) Show Material materials with Thermal conductivity of 28.1 W/(m·K) | ||

1000.0 °C | 29.9 W/(m·K) Show Material materials with Thermal conductivity of 29.9 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.09E-6 Ω·m Show Material materials with Electrical resistivity of 1.09E-6 Ω·m |

100.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

200.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

300.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

400.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

500.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

600.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

700.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

800.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

900.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

1000.0 °C | 1.16E-6 Ω·m Show Material materials with Electrical resistivity of 1.16E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.3 % Show Material materials with Aluminium of 0.3 % |

Carbon | 0.08 - 0.15 % Show Material materials with Carbon of 0.08 - 0.15 % |

Chromium | 18 - 21 % Show Material materials with Chromium of 18 - 21 % |

Cobalt | 5 % Show Material materials with Cobalt of 5 % |

Copper | 0.5 % Show Material materials with Copper of 0.5 % |

Iron | 5 % Show Material materials with Iron of 5 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Nickel | 65.4 % Show Material materials with Nickel of 65.4 % |

Phosphorus | 0.02 % Show Material materials with Phosphorus of 0.02 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 0.2 - 0.6 % Show Material materials with Titanium of 0.2 - 0.6 % |